Int. J. Electrochem. Sci., 12 (2017) 9994 – 10002, doi: 10.20964/2017.11.83
International Journal of
Construction of TiO2
/Si Heterostructure by Nanoepitaxial Growth of
Liguo Gao1,*, Yanqiang Li1, Qun Li1, Hanlin Chen1, Tingli Ma2,* 1
State Key Laboratory of Fine Chemicals, School of petroleum and chemical engineering, Dalian University of Technology, Panjin, 124221, China.
Graduate School of Life Science and Systems Engineering, Kyushu Institute of Technology, 2–4 Hibikino, Wakamatsu, Kitakyushu, Fukuoka 808–0196, Japan.
E-mail: email@example.com, firstname.lastname@example.org
Received: 15 August 2017 / Accepted: 22 September 2017 / Published: 12 October 2017
Nearly defect-free interfaces can be formed using two lattice-matched semiconductors and nanoepitaxial growth methods that can be controlled at the atomic level. In this work, the nanoepitaxy of anatase-type TiO2 on crystalline silicon substrates for fabricating TiO2/Si heterogeneous interface is demonstrated by combining self-assembly and hydrothermal methods. Solid-phase nanoepitaxy is formed in this heterogeneous interface according to the crystal type and crystal lattice matching between anatase-type TiO2 and crystalline silicon. X-ray diffraction (XRD) and crystal symmetry indicate that the nanoepitaxy growth of anatase-type TiO2 on the Si (001) plane is (001) plane. Anatase-type TiO2 atoms are directly connected with Si atoms. Inconsiderable SiO2 exists between anatase-type TiO2 and crystalline silicon substrate. These interfaces could promote the transfer rate of carriers and decrease the recombination rate of hole–electron pairs. This evidence is confirmed by comparison with rutile-type TiO2, which could not be grown on Si substrate due to the mismatching crystal lattice parameter. The rutile-type TiO2 can be removed easily in ultrasonic condition.
Keywords: heterogeneous interface; crystal type and lattice matching; crystal induced; nanoepitaxial growth
capacity and ferroelectric properties at the interface. Construction methods of heterogeneous interface connection can be divided into three types: bridging linker, layer-by-layer assembly, and synthesis of nanocrystals in solution or in gas phase. Miljevic et al. combined Au and TiO2 nanocrystals through bridging linker method by using bifunctional groups to improve photocatalytic efficiency. Yamada et al. deposited nanocrystal CeO2 onto the surface of Pt nanoparticles by layer-by-layer assembly method and prepared a heterogeneous interface with CeO2- onn ion hi h in i l i i i n l l. combined PbTe of epitaxial growth and PbS that was fabricated by the epitaxial growth of PbTe on PbS nanocrystals in solution, thereby forming a PbTe–PbS core/shell nanocomposite with high electric conductivity and low thermal conductivity.
Heterogeneous interface is crucial to the design of PEC devices. Semiconductor silicon is used as the substrate, and a metal-oxide-semiconductor heterogeneous interface is constructed, which will serve as transistor and interface for PEC water splitting.[17–20] Common metallic oxides include Mg2Al2O4, MgO, and TiO2[18,23]. However, the existence of SiO2 on silicon surface forms a large potential barrier against passing through of electrons and restricts the electron–hole transfer at the interface. Therefore, direct nanoepitaxial growth on silicon surface can effectively reduce the electron– hole combination on the interface and increase the transfer rate of carriers, thereby improving the photoelectric property. Li et al. reported that the lattice constant of cubic perovskite SrTiO3 matches well with the Si(001) surface unit cell and developed nearly defect-free interfaces successfully on the silicon surface through the epitaxial growth of molecular beam. Sahasrabudhe et al. connected one layer of amorphous TiO2 on the silicon surface of H:Si under vacuum and low-temperature conditions through a series of vapor depositions.
Research has proven that anatase-type TiO2 crystal possesses higher electron–hole transfer capacities than amorphous TiO2 does.[25,26] In this study, anatase-type TiO2 growth is induced on the (001) surface of n-type monocrystalline Si by layer-by-layer assembly method and nanoepitaxial growth. Anatase-type TiO2 can be directly grown on the silicon surface due to the two lattice-matched semiconductors. Comparison with the synthesis experiments of rutile nanorod on silicon surface confirm that only anatase-type TiO2 with matched crystal type and lattice can grow on silicon surface. The PEC test indicates that the prepared TiO2/Si sample has basically the same onset potential and saturation photocurrent density as monocrystalline Si.
2. EXPERIMENTAL SECTION
2.2 Preparation of Silicon Substrates
Silicon wafer was cut into 1.5*1.5 cm2 slices and washed in an ultrasonic bath (240 W) with acetone, chloroform, ethanol, deionized (DI) water about 5 min, respectively. Then, Si wafers was soaked in a 1:1:5 (by volume) solution of ammonia solution (25%), hydrogen peroxide (H2O2, 30%) and DI water for 60 min at 80℃. They are washed in an ultrasonic bath with DI water for 5 min. To remove SiO2, Si wafers were put in a 3:1 (by volume) solution of H2O, and hydrogen fluoride (40%) for 5 min. They were put into ethanol absolute rapidly after removing SiO2.
2.3 Nanoexpitaxial of Anatase-type TiO2
For nanoepitaxial growth anatase-type TiO2 process, the Si wafers were firstly dipped in titanium tetrachloride for 1 min. Then, they were washed in ultrasonic bath with DI water for 1 min. A clean process with ethanol solution was carried out before dipping the Si wafers into titanium tetrachloride again. This progress was prepared by repeating eight times from dipping in titanium tetrachloride to washing with ethanol solution to grow a connecting layer on Silicon substrate. Glacial acetic, tetrabutyl titanate and DI water with a volume ratio of 30:0.5:0.4 was added in Teflon-lined autoclave and heated at 140℃ for 8 h. After the hydrothermal process, the samples were collected and washed with DI water. Finally, the samples were annealed at 250℃ for 2 h with 5℃/min heating rate in N2 atmosphere. Then, they cooled at room temperature.
2.4 Nanoexpitaxial of Rutile-type TiO2
For nanoepitaxial growth rutile-type TiO2 process, the Si wafers were firstly dipped in titanium tetrachloride for 1 min. Then, they were washed in ultrasonic bath with DI water for 1 min. A clean process with ethanol solution was carried out before dipping the Si wafers into titanium tetrachloride again. This progress was prepared by repeating eight times from dipping in titanium tetrachloride to washing with ethanol solution. Hydrochloric acid (15 mL, 6M) was well dissolved into 15 mL DI water under magnetic stirring to get solution A. Then, 0.5 mL tetrabutyl titanate was taken using the pipetting to dissoved into the above solution to get solution B. The Silicon substate and solution B were added in Teflon-lined autoclave and heated at 150℃ as reported by others. After the hydrothermal process, the samples were collected and washed with DI water. Finally, samples were annealed at 250℃ for 2 h with 5℃/min heating rate in N2 atmosphere. Then, they cooled at room temperature.
2.5 Preparation of anatase-type TiO2 (Spin-coating)/Si
tetrachloride again. This progress was prepared by repeating eight times from dipping in titanium tetrachloride to washing with ethanol solution to grow a connecting layer on Silicon substrate. A compact TiO2 agent was spin-coated onto the Si substrates, which were sequentially annealed at 450 °C for 30 min.
2.6 Catalyst Ni deposited
Ni film was deposited onto TiO2/Si substrates by a thermal deposition process. During the deposition process, the system was maintained under a pressure of 10-4 Pa and at a rate of 0.03 Å/S. Ohmic contacts to the back sides of TiO2/Si samples were formed by evaporating Ag onto the unpolished surface with 20 nm thicknesses.
The surface morphology was determined by SEM on a Nova NanoSEM 450 (FEI). The lattice structure was observed under a HRTEM at an accelerating voltage of 200 kV (HRTEM, Tecnai G2 F20). The chemical compositions of the samples were analyzed by EDS, which is equipped on HRTEM. The crystal structure of the samples were studied by XRD (XRD-7000S) using Cu KR radiation from 20° to 80° at a scanning speed of 5°/min. All electrochemical experiments were performed on CHI630D electrochemical work station in air at room temperature. All electrolyte solutions prepared with DI water. A saturated calomel electrode was used as the reference electrode. Pt wire was used as the counter electrode for all electrochemical measurements performed in 1.0 M KOH (aq) electrolyte. The linear sweep voltammetry curves were measured at 100 mV/S without iR compensation. During the measurement, the electrolyte was vigorously stirred with a magnetic stir bar driven by a model-train motor. A Xenon arc lamp was used as the light source. Illumination was provided by an AM 1.5G solar simulator, and the intensity was adjusted to 100 mW/cm2 by the standard silicion cell. All the electrodes in this study were typically 0.2 cm2 in area. All measured potentials were converted to the NHE reference scale using E(NHE)= E(SCE)+0.2415V.
3. RESULTS AND DISCUSSION
TiO2 on monocrystalline Si surface is possible. Studies have shown that only crystals with matched lattice and crystal form can be crystal-face-induced nanoepitaxial grown. Hojo et al. demonstrated well-aligned heterogeneous interfaces by selectively nucleating anatase-type TiO2 in a one-on-one fashion and grown epitaxially on a nanocrystalline monolayer of CeO2. The anatase-type TiO2 grew uniformly along the  direction on the (001) surfaces of CeO2 nanocubes. Strontium titanate, SrTiO3, can be grown epitaxially on Si (001) with minimal interfacial reactions. The lattice constant of a cubic perovskite SrTiO3 (3.905 Å) matches well with the Si (001) surface unit cell (3.84 Å), which results in a small (–1.7%) lattice mismatch with SrTiO3/Si and low interface state density. It creates a nearly perfect electrical interface. Ji et al. revealed a thin epitaxial layer of SrTiO3 grew directly on Si(001) by molecular beam epitaxy to form an metal–insulator–semiconductor photocathode, where the photogenerated electrons can be transported easily through SrTiO3 layer and result in a high photon-to-current efficiency.
Figure 1. Schematic crystal structure (a) Si unit cell; (b) Anatase-type TiO2 unit cell
Figure 2. (a) SEM image of Anatase-type TiO2 nanoepitaxy on Si substrate, the insert is HRTEM profile image of TiO2/Si heterogeneous interface; (b) XRD pattern of Si, Si/TiO2 and TiO2
The induction of rutile-type TiO2 by monocrystalline Si is compared in this study to further verify that anatase-type TiO2 and monocrystalline Si have matched crystal type and lattice and only crystals with matched lattice and crystal form can be crystal-face-induced nanoepitaxial grown. The growth period of rutile-type TiO2 is shown in Fig. 3. Rutile-type TiO2 is rod crystal, and rod-shaped TiO2 grows gradually on the side as the hydrothemal synthesis continues, thereby forming flower-like TiO2. The XRD analysis shown in Fig. 3d proves that the prepared rod-shaped TiO2 is rutile-type TiO2 and that its characteristic peak is at θ=27 4°. The lattice constants of the unit cell of rutile are a=b=0.4594 nm and c=0.2959 nm, which disagree with those of monocrystalline Si. Therefore, rutile cannot have nanoepitaxial growth on monocrystalline Si. The nanorod rutile-type TiO2 in Fig. 3a is also easy to be peeled off from the monocrystalline Si surface by ultrasonic processing.
Figure 4. SEM image of rutile-TiO2 nanorod on Si substrate, (a) without ultrasonic treatment; (b) with ultrasonic treatment; the insert is a magnified SEM image of anatase-type TiO2.
Anatase-type TiO2 still could be seen on the silicon surface after nanorod rutile-type TiO2 is peeled off by ultrasonic processing shown in Fig. 4. This anatase-type TiO2 grows at the silicon substrate surface by crystal induction and cannot be removed by ultrasonic processing. The amplification illustration in Fig. 4b depicts that this square TiO2 is different from nanorod rutile-type TiO2 and has not been reported yet. Hence, although rutile-type TiO2 is the precondition for TiO2 synthesis, anatase-type TiO2 still could grow on silicon surface due to the induction of monocrystalline Si surface. However, the anatase-type TiO2 is square and has a small quantity.
same onset potential and photocurrent density. The applied voltage at the maximum photocurrent is relatively high, which is related to the TiO2 film thickness. In other words, the PEC properties of Si change slightly after the nanoepitaxial growth of TiO2. Therefore, the TiO2/Si heterostructure can use TiO2 to protect Si and avoid corrosion of monocrystalline Si in solution without influencing Si properties. This heterostructure has great application potentials in the photoanode of PEC water splitting.
Nanoepitaxial growth of TiO2 of anatase-type TiO2 on the (001) surface of monocrystalline Si is achieved by combining layered self-assembly and hydrothermal synthesis, which is attributed to their lattice and crystal type matching. The conditions for growth of nanorod rutile-type TiO2 prove that lattice and crystal type matching are the preconditions for nanoepitaxial growth of crystal heterogeneous interface; otherwise, nanoepitaxial growth is impossible, and the heterogeneous interface is easy to be peeled off from the surface. Nanoepitaxial growth TiO2 on monocrystalline Si surface has high transfer capacity of carriers and basically the same PEC properties with monocrystalline Si. Its saturation photocurrent density is 20 times higher than that of TiO2 (Spin-coating)/Si substrate.
This work was financially supported by the Fundamental Research Funds for the Central Universities (Grant No. DUT16QY04), the National Natural Science Foundation of China (Grant No. 51273032 and 91333104).
1. J.W. Reiner, A.M. Kolpak, Y. Segal, K.F. Garrity, S. m il‐B igi C.H. Ahn, and F.J. Walker, Adv. Mater., 22 (2010) 2919.
2. D. K. Fork, D.B. Fenner, G.A.N. Connell, J.M. Phillips, and T.H. Geballe, Appl. Phys. Lett., 57 (1990) 1137.
3. J.M. Bao, Nature. Nanotech., 10 (2015) 19.
4. D. Hojo, T. Togashi, T. Ohsawa, M. Saito, Z.C. Wang, Y. Sakuda, S. Asahina, Y. Ikuhara, T. Hitosugi, and T. Adschiri, Cryst. Growth Des., 14 (2014) 4714.
5. H.L. Chen, H.C. Cheng, T.S. Ko, S.Y. Chuang, and T.C. Chu, Jpn. J. Appl. Phys., 45 (2006) 6984. 6. G.A. Sotiriou, A.M. Hirt, P.Y. Lozach, A. Teleki, F. Krumeich, and S.E. Pratsinis, Chem. Mater.,
23 (2011) 1985.
7. A. Tanaka, A. Ogino, M. Iwaki, K. Hashimoto, A. Ohnuma, F. Amano, B. Ohtani, and H. Kominami, Langmuir, 28 (2012) 13105.
8. H. Yu, M. Chen, P.M. Rice, S.X. Wang, R.L. White, and S. Sun, Nano lett., 5 (2005) 379. 9. X.L. Sun, N.F. Huls, A. Sigdel, and S.H. Sun, Nano lett., 12 (2012) 246.
10.T.D. Schladt, T. Graf, O. Köhl H Bauer, M. Dietzsch, J. Mertins, R. Branscheid, U. Kolb, and W. Tremel, Chem. Mater., 24 (2012) 525.
12.L. Ji, M.D. McDaniel, S.J. Wang, A.B. Posadas, X.H. Li, H.Y. Huang, J.C. Lee, A.A. Demkov, A.J. Bard, J.G. Ekerdt, and E.T. Yu, Nature Nanotech., 10 (2015) 84.
13.M. Miljevic, B. Geiseler, T. Bergfeldt, P. Bockstaller, and L. Fruk, Adv. Funct. Mater., 24 (2014) 907.
14.Y. Yamada, C.K. Tsung, W. Huang, Z. Huo, S.E. Habas, T. Soejima, C.E. Aliaga, G.A. Somorjai and P. Yang, Nat. Chem., 3 (2011) 372.
15.M. Ibáñez, R. Zamani, S. Gorsse, J. Fan, S. Ortega, D. Cadavid, J.R. Morante, J. Arbiol, and A. Cabot, ACS nano, 7 (2013) 2573.
16.K. Eisenbeiser, J.M. Finder, Z. Yu, J. Ramdani, J.A. Curless, J.A. Hallmark, R. Droopad, W.J. Ooms, L. Salem, S. Bradshaw, and C.D. Overgaard, Appl. Phys. Lett., 76 (2000) 1324.
17.K. Sun, S. Shen, J.S. Cheung, X. Pang, N. Park, J. Zhou, Y. Hu, Z. Sun, S.Y. Noh, C.T. Riley, P.K.L. Yu, S. Jin, and D. Wang, Phy. Chem. Chem. Phys., 16 (2014) 4612.
18.Y.W. Chen, J.D. Prange, S. Dühnen, Y. Park, M. Gunji, C.E.D. Chidsey, and P.C. McIntyre, Nat. Mater., 10 (2011), 539.
19.K. Sun, X. Pang, S. Shen, X. Qian, J.S. Cheung, and D. Wang, Nano lett., 13 (2013) 2064.
20.J. Feng, M. Gong, M.J. Kenney, J.Z. Wu, B. Zhang, Y. Li, and H. Dai, Nano. Res., 8 (2015) 1577. 21.M. Ihara, Y. Arimoto, M. Jifuku, T. Kimura, S. Kodama, H. Yamawaki, and T. Yamaoka, J.
Electrochem. Soc., 129 (1982) 2569.
22.D.K. Fork, F.A. Ponce, J.C. Tramontana, and T.H. Geballe, Appl. Phys. Lett., 58 (1991) 2294. 23.M.T. McDowell, M.F. Lichterman, A.I. Carim, R. Liu, S. Hu, B.S. Brunschwig, and N.S. Lewis,
Appl. Mater. Inter., 7 (2015) 15189.
24.G. Sahasrabudhe, S.M. Rupich, J. Jhaveri, A.H. Berg, K.A. Nagamatsu, G. Man, Y.J. Chabal, A. Kahn, S. Wagner, J.C. Sturm and J. Schwartz., J. Am. Chem. Soc., 137 (2015) 14842.
25.A.G. Scheuermann, J.P. Lawrence, A.C. Meng, K. Tang, O.L. Hendricks, C.E.D. Chidsey and P.C. Mclntyre, Appl. Mater. Inter., 8 (2016) 14596.
26.B. Ohtani, Y. Ogawa, and S.J. Nishimoto, J. Phys. Chem. B, 101 (1997) 3746.
27.M.P. Warusawithana, C. Cen, J.C. Woicik, Y. Li, L.F. Kourkoutis, J.A. Klug, P. Ryan, L.P. Wang, M. Bedzyk, D.A. Muller, L.Q. Chen, J. Levy, and D.G. Schlom, Science, 324 (2009) 367.
28.R.A. McKee, F.J. Walker, and M.F. Chisholm, Science, 293 (2001) 468. 29.Y. Xing, and X. Ding, J. Appl. Polym. Sci., 103 (2007) 3113.
30.J. Cai, J. Ye, S. Chen, X. Zhao, D. Zhang, S. Chen, Y. Ma, S. Jin, and L. Qi, Energ. Environ. Sci., 5 (2012) 7575.